**HAL Id: hal-01004927**

**https://hal.archives-ouvertes.fr/hal-01004927**

### Submitted on 11 Jun 2014

**HAL is a multi-disciplinary open access**

### archive for the deposit and dissemination of

### sci-entific research documents, whether they are

### pub-lished or not. The documents may come from

### teaching and research institutions in France or

### abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**

### destinée au dépôt et à la diffusion de documents

### scientifiques de niveau recherche, publiés ou non,

### émanant des établissements d’enseignement et de

### recherche français ou étrangers, des laboratoires

### publics ou privés.

### Public Domain

**A numerical analysis of the evolution of bundle**

**orientation in concentrated fibre-bundle suspensions**

### Pierre J.J. Dumont, Steven Le Corre, Laurent Orgéas, Denis Favier

**To cite this version:**

### Pierre J.J. Dumont, Steven Le Corre, Laurent Orgéas, Denis Favier. A numerical analysis of the

### evolution of bundle orientation in concentrated fibre-bundle suspensions. Journal of Non-Newtonian

### Fluid Mechanics, Elsevier, 2009, 160 (2-3), pp.76-92. �10.1016/j.jnnfm.2009.03.001�. �hal-01004927�

### A numerical analysis of the evolution of bundle orientation in concentrated

### ﬁbre-bundle suspensions

### P.J.J. Dumont

a_{, S. Le Corre}

b,∗_{, L. Orgéas}

c_{, D. Favier}

c
a* _{CNRS/Universités de Grenoble, Laboratoire de Génie des Procédés Papetiers (LGP2), 461 rue de la Papeterie, BP 65, 38402 Saint-Martin-d’Hères cedex, France}*
b

_{GeM - Institut de Recherche en Génie Civil et Mécanique, CNRS/École Centrale de Nantes, BP 92101, 44321 Nantes cedex 3, France}c_{CNRS/Universités de Grenoble, Laboratoire Sols-Solides-Structures-Risques (3S-R), BP 53, 38041 Grenoble cedex, France}

*Keywords:*

Highly concentrated ﬁbre suspensions Fibre orientation distribution function Micro–macro modelling

Computational rheometry

The rheology of Newtonian concentrated ﬁbre-bundle suspensions with nearly planar orientation states
is investigated within the framework of the homogenization method for periodic discrete structures.
These suspensions are seen as forming a connected network of bundles. At their contact points, the ﬂow
induces local Newtonian interaction forces and moments. “Numerical rheometry experiments” are
per-formed on representative elementary volumes of these suspensions to explore the inﬂuence of bundle
volume fraction and orientation state on the rate of change of bundle orientation. Three bundle
orien-tation distributions are particularly investigated: Gaussian-based, uniform and crenellated orienorien-tation
*distributions. Two types of numerical simulations are performed, i.e., instantaneous and time-evolution*
ones. The obtained numerical results permit to discuss the role of the shape of the orientation
distri-bution, typically on the rate of change of the second-order orientation tensor. They are also compared
to the well-known Jeffery theory and its subsequent modiﬁcations like the Folgar–Tucker theory. The
accuracy of some well-known closure approximation functions of the fourth-order orientation tensor is
examined. It appears that, in the case treated here where the suspending ﬂuid and the ﬁbre–ﬁbre
inter-actions are Newtonian, the Jeffery’s equation gives a fairly good ﬁt (the best ﬁt of all examined theories)
of the homogenization results, despite the completely different physics of both approaches. Some
dif-ferences are observed in situations where ﬁbre-bundles are highly aligned along the ﬂow direction. It is
also observed that the shape of the orientation distribution strongly affects the rate of the orientation
change. At last, the tested closure approximations can lead to good description of some particular cases of
orientation distributions. Nonetheless, in general cases, they are not relevant at all so that other strategies
would have to be used in order to compute the evolution of ﬁbre orientation.

**1. Introduction**

Polymer composites reinforced with short ﬁbre-bundles[1–3] are increasingly used in many industrial processes to produce parts having complex shapes, due to their lightweight and cost-effective properties. The main issue for these materials is to control the ﬁbre content homogeneity and the ﬁbre-bundle orientation induced by the forming processes. Practical applications for structural parts involve highly concentrated suspensions (typical volume fraction of ﬁbres ≈10–30%), where short range bundle–bundle interac-tions given by relative motion at bundle–bundle contacts are not negligible and can even be regarded as the dominating physical mechanism[4–7].

This observation is the starting point of the approach presented here, which has already been developed and validated in

previ-∗ Corresponding author. Tel.: +33 2 40 37 25 27; fax: +33 2 40 37 25 66.

*E-mail address:*steven.le-corre@ec-nantes.fr(S. Le Corre).

ous papers[6,7]. In Le Corre et al.[6], a theoretical framework was
developed to obtain the mechanical behaviour of a planar network
of ﬁbre-bundles using the homogenization technique for periodic
discrete structures. In Le Corre et al.[7], efforts aimed at (i)
propos-ing a simple acceptable local bundle–bundle interaction model,
(ii) developing numerical simple schemes to mimic real networks
of ﬁbre-bundles and to compute their macroscopic behaviour and
(iii) comparing the prediction of the micro–macro model with the
rheological experiments performed on a non-linear viscous planar
*suspension, i.e. an industrial Sheet Moulding Compounds (SMC).*

Another observation is that numerical simulation works, which
aim at predicting the ﬁbre orientation evolution occurring during
the ﬂow of this type of industrial concentrated suspensions,
are commonly but quite surprisingly based on theories whose
*domains of validity are a priori restricted to dilute or semi-dilute*
suspensions[8,9]. The models based on this approach are obtained
from the well-known Jeffery’s equation[10]for a remote ﬁbre in
a Newtonian ﬂuid. This model can be modiﬁed in order to account
for hydrodynamic interactions between ﬁbres by involving the

modiﬁcations proposed by Tucker and Advani [8]. Usually, this approach leads to describe the evolution of ﬁbre orientation by an equation for the rate of the second-order orientation tensor. This equation has the drawback to include the fourth-order orientation tensor and consequently raises the underlying problem of choos-ing an appropriate closure approximation to solve the problem. Here the main issue is to investigate the relevance of this type of approach for concentrated suspensions of ﬁbre-bundles.

Hence three ways are followed along this study. Firstly, the
pre-dictions of the commonly used models (Jeffery and Folgar Tucker
type theories) for ﬁbre orientation evolution are compared with the
direct calculation results provided by the presented micro–macro
approach. Secondly, the inﬂuence of the shape of the ﬁbre
ori-entation distribution on the rate of the oriori-entation evolution is
*quantiﬁed: i.e., a broad spectrum of concentrated suspensions,*
which may exhibit three different orientation distributions, are
numerically tested. Thirdly, as it is known that some closure
approx-imations were developed to work for some characteristic ﬁbre
orientation distributions [9], the accuracy of some well-known
closure approximations is examined for all considered
microstruc-tures.

For that purpose, a non-exhaustive review of commonly used
ﬁbre orientation models, based on Jeffery’s work, is given in Section
2. In Section3, a brief presentation of the micro–macro approach,
which has been extensively developed in[6,7], is achieved. Some
details are given on the numerical technique used to generate
the Representative Elementary Volumes (REV’s) of the
stud-ied suspensions, in particular on the three different considered
*ﬁbre orientation distributions, i.e., Gaussian-based, uniformly *
dis-tributed and crenellated. Furthermore, the principle of calculations
performed to compute the evolution of the ﬁbre-bundle orientation
is explained. Then instantaneous simulation results are presented
in Section4in order to discuss the inﬂuence of the ﬁbre volume
fraction and the role of the current orientation state on the rate
of the second-order orientation tensor. These results are compared
with predictions of the common theories. The same type of
com-parison is also performed for time-evolution calculations under
homogeneous mechanical loading conditions in Section5.

**2. State of the art in ﬁbre orientation modelling**
*2.1. Motion of a single ﬁbre immersed in a Newtonian ﬂuid*

Jeffery’s theory[10]forms the basis of most current approaches
to describe ﬁbre suspension rheology and in particular ﬁbre
ori-entation modelling. One of the main contribution of this theory
**consists in giving an expression for the angular velocity ω of an**
ellipsoidal particle in an incompressible inﬁnite Newtonian
sus-pending ﬂuid with no external forces or torques. Later, Hand[11]
compared and showed that the Jeffery equation is a special case of
a more general equation obtained by Ericksen[12]in his
invariant-based theory of anisotropic ﬂuid (the so-called TIF theory) for the
**evolution of an unit vector p, characterizing a preferred direction**
**at each material point x of the ﬂuid. If the main axis of revolution**
**of the ellipsoidal particle is described by this unit vector p and if**
we consider the cylindrical shape being an approximation to the
ellipsoid, the following Jeffery–Ericksen equation may be used to
describe the motion of the ﬁbre:

**˙p= ω × p = .p + (D · p − (p · D · p)p) ,** (1)

**where ˙p denotes the material derivative of p, is the shape factor**
of the ﬁbre ( = (r2_{− 1)/(r}2_{+ 1) with r = l/d the ﬁbre aspect ratio}
*where l and d are respectively the length and the diameter of the*
**ﬁbre), the vorticity tensor and D the strain rate tensor, i.e., the****skew-symmetric and symmetric parts of the velocity gradient L**=

**grad**

**v**

, respectively, with**v**

**v**

the ﬂuid velocity.
**v**

*2.2. Evolution equation for the orientation distribution function *

In the case of a suspension of ﬁbres, a reasonable way to describe
the orientation of ﬁbres and its evolution consists in adopting a
global statistical approach at each material point. For that purpose,
**the distribution function of orientation , as a function of x, p, and**

**t, can be used. At each material point x, the elementary probability***dP of ﬁnding a ﬁbre whose orientation is located in the portion of*

*space delimited by the elementary solid angle dp is written as*

**dP = (x, p, t) dp.** (2)

**The distribution function is -periodic: (x, p, t) = (x, −p, t). It**
is normalized so that the probability of an orientation on the whole
orientation space is unity:

** (x, p, t) dp = 1.** (3)

The evolution equation of has the following alternative forms [13]: d dt + di

*v*

**p( ˙p)**= 0, (4) where d dt = ∂ ∂t +

**v**

**v**

**· gradx + ˙p · gradp**. (5)

**If the following notation is adopted D /Dt = (d /dt) − ˙p · gradp** ,
Eq.(4)writes:

D

Dt + di

*v*

**p( ˙p) = 0.**(6)

Following Dupret and Verleye[9]**, ˙p can be expressed by a **
**con-stitutive equation, which is a function of p. For instance, the Jeffery**
equation, whose assumptions are very restrictive, is applicable to
describe the evolution of the orientation of ﬁbres contained in
dilute suspensions, where hydrodynamic interactions of long and
short range between ﬁbres can be considered as negligible.

*2.3. Evolution equation for the second-order orientation tensor*

Determining the orientation state by solving the evolution
**equa-tion for is quite cumbersome since (x, p, t) has six independent**
variables in the 3D case and this task asks for heavy
calcula-tions. This is why orientation tensors were introduced. Orientation
*tensors are obtained by averaging the n th dyadic products over*
orientation space, with as the weighting function[14]. Due to
the normalization and the periodicity of , the odd-order
orienta-tion tensors are all zero. Usually only the second and fourth-order
orientation tensors are used. They are deﬁned as follows:

**A**(2)=

**p⊗ p (p) dp,**(7)

**A**(4)=

**p⊗ p ⊗ p ⊗ p (p) dp.**(8)

* These tensors only depend on space x and time t variables. It is then*
easy to show that the time-evolution equation of the second-order
orientation tensor using(4)writes:

**˙A**(2)=

**{ ˙p ⊗ p + p ⊗ ˙p} (p) dp.** (9)

**Injecting for instance the form of ˙p**_{J}given by Eq.(1)provides the
**following equation for ˙A**(2):

**˙A**(2)**= · A**(2)
**− A**(2)
**· + (A**(2)
**· D + D · A**(2)
**− 2A**(4)
**: D).** (10)

**Notice that, given the imposed macroscopic velocity gradient L**=

**grad**

**v**

**v**

**, the above equation implies that ˙A**(2)

**is a linear function of L.**In particular, we have:

**˙A**(2)(**−L) = − ˙A**(2)**(L).** (11)

The evolution equation of the second-order orientation tensor has the drawback to involve the fourth-order orientation tensor

**A**(4). This difﬁculty is usually circumvented by deﬁning a closure
**approximation expressing A**(4) **in terms of A**(2). This problem has
led to several developments by different authors which ﬁrst can
be found in a paper of Prager[15]. A large variety of closure forms
are reviewed in some papers by Advani and Tucker[16]and Dupret
and Verleye[9]or Doghri and Tinel[17]. Among the different closure
approximations, we will examine in this paper the linear[18,14], the
quadratic[19], the hybrid[14]and the natural[9]closure
*approx-imations. They are detailed below in their 2D forms, i.e., for ﬁbre*
**orientation contained in a plane (e**1, e2), using indicial notations
(i, j, k, l ∈ {1, 2}):

• Linear closure approximation[18,14]:
A(4)L_{ijkl} = − 1

24(ıijıkl+ ıikıjl+ ıilıjk) +1

6(Aijıkl+Aikıjl+Ailıjk+Aklıij+Ajlıik+Ajkıil), (12) • Quadratic closure approximation[19]:

A(4)Q_{ijkl} = A(2)
ij A

(2)

kl , (13)

• Hybrid closure approximation[14]:
A(4)H_{ijkl} **= 4 det A**(2)

A(4)linear_{ijkl} **+ (1 − 4 det A**(2)

)A(4)quadratic_{ijkl} , (14)
• Natural closure approximation[9]:

A(4)N_{ijkl} = 1

3(AijAkl+ AikAlj+ AilAjk)+16**det A**
(2)

(ıijıkl

+ ıikılj+ ıilıjk). (15)

*2.4. Models of hydrodynamic interactions between ﬁbres*

In order to take into account ﬁbre–ﬁbre hydrodynamic
inter-actions in semi-dilute suspensions and to provide a constitutive
**equation for the material derivative ˙p, Jeffery’s equation can be**
modiﬁed as follows:

**˙p= ˙p**J**+ q**d, (16)

**where ˙p**_{J}is given by(1)**and q**_{d}is a term, which concept in the case
of non-Brownian ﬁbre suspension has been ﬁrst proposed by
Fol-gar and Tucker[13]and later modiﬁed and called by Rahnama et
al.[20]“orientational dispersion ﬂux”. Detailed analyses of the
ran-domization effects of this term on the ﬁbre orientation distribution
are given in different studies by Shaqfeh and Koch[21,22]and
Rah-nama et al.[20]for shear and uniaxial ﬂow kinematics. A general
form for this term is proposed by Koch[23]and Petrich et al.[24]:

**q**d_{= −Dr}_{· grad}

**p** , (17)

**where tensor D**r is called the orientational diffusion tensor.
Dif-ferent isotropic and anisotropic forms of this diffusion term are
proposed. For instance, Folgar and Tucker[13]have ﬁrst suggested
an isotropic diffusion term:

**D**r= Dr**ı** with Dr= CI˙, (18)

where CI is the interaction coefﬁcient, which needs to be
deter-mined from experiments or simulation results (see for instance
[25,26]or[27]) and ˙ =√**2D : D the generalized shear strain rate**

of the ﬂuid. Some anisotropic diffusion terms have also been pro-posed. For example, the one given by Fan et al.[28]reads:

**D**r**= C ˙,** (19)

**where C is a second-order symmetric tensor, which components**
have to be determined experimentally.

In the case of isotropic diffusion, the form of the equation for
**˙A**(2)is consequently modiﬁed as follows[14]:

**˙A**(2) **= .A**(2)** _{− A}**(2)

**. + **

**A**(2)

**.D + D.A**(2)

**− 2A**(4)

**+ 2Dr**

_{: D}**(ı− ˛A**(2)

), (20)

with ˛ = 2 or 3, respectively in 2D or 3D ﬁbre orientation. To the
best of our knowledge, it must be pointed out that all these forms
**for D**rbreak the linearity(11)**of ˙A**

(2)

**with respect to L.**

**3. The present micro–macro approach**

This section summarizes the micro–macro model developed in [6,7]to model the rheology of highly concentrated ﬁbre-bundle suspensions with planar bundle orientation.

*3.1. Micromechanical model and upscaling*

*The considered suspensions are sheets of thickness h in which*
*slender ﬁbre-bundles of length l (h < l) are immersed in an*
incompressible Newtonian ﬂuid. These bundles form connected
*networks, i.e., with no isolated bundle or group of bundles. *
Bun-dles have elliptical cross-section dmaxdmin/4, which main axis
dmax( dmin) is contained in the plane of the sheets* P ≡ (e*1, e2).

*The thickness h being small compared to l, it will be assumed*

*that each bundle b has a main and mean orientation along a unit*

**vector p**

_{b}= cos b

**e**1+ sin b

**e**2 contained in

*P*[29,30]. This does not mean that bundles are straight: indeed, because of the very

*high bundle content f (0.05 < f < 0.3) and h < l, bundles may be*initially slightly bent or wavy around their major axis dmax. Like-wise, since dmax dmin, we will (i) neglect bending efforts in the thickness of the sheet, and (ii) neglect the bending of the bun-dle in

*P. The last assumption is similar to the one stated in*[7,5]. It is supported by experimental evidences. Observations on indus-trial[3,29]and model[30]concentrated planar bundle suspensions show that the small axis dminof bundles’ cross-section in these

**sus-pensions are aligned in the e3-direction. Furthermore, bundles are**highly compliant compared with “classical” ﬁbres: they can bend

**and ﬂatten along e**3without any signiﬁcant effort, at least within the investigated strain range. Therefore, this justiﬁes the presented simple micromechanical model for the interactions between

**bun-dles where forces in the e**3-direction are neglected. This leads also to the two following consequences:

*(a) The motion of a bundle b inP is simply given by the translational*

˜

**v**

band angular ˙b**v**

**e**3 velocities of the centre of mass Gbof the

**bundle (˜x being the projection of x in**

*P). Moreover, the*

out-of-plane shearing at the macroscale has not been studied: noting

**L= grad**

**v**

, respectively, with**v**

**v**

the macroscopic velocity
gradi-ent of the suspension, only situations for which Li3= L3i= 0
(i = 1, 2) are explored.
**v**

(b) As explained in Le Corre et al.[7], it is assumed that during the deformation of the suspension, contacting bundles inter-act with forces and local moments induced by the shearing of a small amount of a ﬂuid entrapped in contact zones. As the suspensions under consideration are very concentrated, such deformation mechanisms are supposed to be the main mechan-ical contributions to the overall stress of the suspension. In this paper, the entrapped ﬂuid is simply considered as Newtonian,

**Fig. 1. Modelling of bundle–bundle interactions: (a) view of a connection between two neighbouring ﬁbre-bundles, (b) side view of the sheared zone, (c) top view of the**

surface of the sheared zone.

its viscosity being that of the suspending ﬂuid. Concerning
this last point, very simple assumptions are stated to model the
geometry and the mechanics of the entrapped ﬂuid: at a given
*contact zone k between bundles b and c, of centre K, such a*
complex situation is assumed to be equivalent to the shearing
of thin prism of height ˛, which in-plane dimensions and
orien-tation depend on dmax**, the orientation of the bundles p**_{b}**and p**_{c},
as well as the relative orientation of the bundles k(seeFig. 1).
*During the relative motion of b and c, the entrapped Newtonian*
ﬂuid is subjected to (i) a simple shear induced by the difference
of in-plane translational velocities ˜

**v**

k= ˜**v**

**v**

c(K) − ˜**v**

**v**

b(K) at point
**v**

* K, and (ii) a torsion along e*3induced by the difference of
angu-lar velocities ˙k= ˙c− ˙b. It is then possible to obtain simple

**estimations of the interaction force ˜f**

_{k}and the local interaction moment Mk(K)e3

*the bundle c exerts on the bundle b*[7]:

**˜f**

_{k}= ˛ d2 max | sin k|˜

**v**

k, Mk(K) =
4
˛
d3
max
| sin k|2 ˙k. (21)
Therefrom, by neglecting acceleration and external volume
forces and moments, by applying the homogenization technique for
discrete periodic structures[31–33], and by assuming that the local
moments Mk**v**

**e**3are small compared to the moments of interaction

**forces ˜f**

_{k}it can be shown that the self-equilibrium of a Representa-tive Elementary Volume (REV) of the suspensions (of volume Vre

*v*)

can be put in the form[6,7]:

### ∀

b ∈ Vre*v*,

### ⎧

### ⎪

### ⎪

### ⎪

### ⎨

### ⎪

### ⎪

### ⎪

### ⎩

*k ∈ C*

_{b}

**˜f**[0]

_{k}

**= 0**

*k ∈ C*

_{b}M

_{k}[0]

**e**3+

*k ∈ C*

_{b}sb

**p**

_{b}

**× ˜f**[0]k

**= 0**(22)

where*C*b*is the set of bundles c connected to bundle b, and sb*is
the local abscissa (from the centre Gb**of b) along p**_{b}of the
*contact-ing point K. In this Eq.*(22)**, ˜f**[0]_{k} and M[0]_{k} represent the ﬁrst-order
**approximations of ˜f**_{k}and Mk**e**3. They are expressed as follows:
**˜f**[0]_{k} =
˛
dmax2
| sin k|˜

**v**

[1]
k , (23)
where
˜**v**

**v**

[1]**v**

_{k}=

**v**

˜[1]c −**v**

**v**

˜[1]**v**

_{b}

**+ ˜L · ˜**k+ sc˙ [0] c

**e**3

**× pc**− sb˙

_{b}[0]

**e**3

**× pb,**(24)

**with ˜**

_{k}

**the projection of GbGc**in

*P, and*

M_{k}[0]=
4
˛
d3
max
| sin k|2( ˙
[0]
c − ˙[0]b ). (25)

In these last equations, ˙_{b}[0]is the ﬁrst-order approximation of ˙b,
ε˜

**v**

[1]**v**

_{b}is the ﬁrst-order ﬂuctuation of ˜

**v**

**v**

_{b}around its ﬁrst-order approx-imation ˜

**v**

[0]**v**

_{b}

**, ˜L= grad˜**

**v**

[0] **v**

_{is the macroscopic velocity gradient,}which is considered as given and imposed for all ﬁbre-bundles con-tained in the REV. Please notice that due to the previous kinematical

*constraints, i.e., incompressibility and Li3*= L3i= 0 (i = 1, 2), this is

**equivalent to impose L. Hence, Eq.**(22)represents a system of 3N

*linear equations with 3N kinematical unknowns, N being the total*number of bundles contained in the REV. It is easily shown from

**(23)–(25) that the unknowns are linear functions of ˜L**[6].

Moreover, the homogenization results show the following prop-erties for the suspensions:

(a) the equivalent continuous medium of the studied suspension
is a Cauchy medium, whose symmetrical macroscopic stress
**tensor is:**
**= −pı + ˜**(f ) _{with} _{}_{˜}(f )_{=} 1
Vre*v*
C

### k=1

**˜**

_{k}

**⊗ ˜f**[0]k , (26)

*ten-sor, Vre*

**where p is the incompressibility pressure, ı the identity***v*

*the volume of the considered REV, C the number of*

bundle–bundle connections in the REV.

(b) the suspension is a linear viscous anisotropic ﬂuid: ˜

(f )**= ˜**(f )_{( ˜}

**D, , microstructure),** (27)

where ˜**D is the strain rate tensor, i.e.. the symmetric part of ˜L.**

Such a theoretical result is a consequence of the previous point (a) and of the system of Eqs.(22)–(25).

(c) at the ﬁrst-order, the rate of change
**˙p**_{b}= ˙[0]

**of any orientation vector p**_{b}**is a linear function of ˜L:**

### ∀

i, j ∈ {1, 2}### ∀

Lij∈ R### ∀

b ∈ Vre*v*

**˙p**_{b}(Lij**e**_{i}**⊗ ej**)= Lij**˙p**_{b}**(e**_{i}**⊗ ej),** (29)

where the Einstein convention has been used for the
*summa-tion on indices i and j. This also a direct consequence of the*
system of Eqs.(22)–(25).

(d) Consequently, the rate of the corresponding distribution
* func-tion and of the n th-order orientafunc-tion tensors A*(n)are also

**linear functions of L. In particular, property**(11)is also veriﬁed.

*3.2. Microstructure generation*

In order to mimic real ﬁbrous microstructures of industrial
polymer composites such as Sheet Molding Compounds (SMC) or
Glass Mat Thermoplastics (GMT), a very simple deterministic
tech-nique directly inspired from the statistical tube model[34–36]
has been developed[7]. Following this tube model, the number
of bundle–bundle contacts per unit volume should be a quadratic
*function of the volume fraction f of bundles. Including the tube*
model in the previous homogenization approach[7]induces that
*the macroscopic extra stress tensor, (e.g., the term ˜*(f ) of the Eq.
(26)) is proportional to the number of contacts in the suspension,
and thus evolves as a quadratic function of the ﬁbre volume fraction

*f. Experimental results*[3,30]depict also such quadratic evolution of
*stress levels with f: this reinforces the relevance of the tube model*
despite its simplicity.

Therefore, this generation process will be used in the following
sections to study the evolution of the orientation of the bundles
*during mechanical loading. Brieﬂy, N bundles (elementary volumes*
dmaxdminl/4) which orientation vectors pbare contained in*P are*
generated inside a 3D REV of volume Vre*v*= d × d × h (seeFig. 2,

*h being the thickness of the REV). The centre of mass G*bof each
bundle has a random position (xb, yb, zb) inside the volume of the
REV.

*The in-plane dimension d of the REV must be chosen larger*
*than the bundle length l, in order to avoid the possibility to *
*gen-erate a continuous ﬁbre-bundle. Practically, d was set to a length*
*1% higher than l, in order to enhance the computation time. Within*
the bundle content range for which the micro–macro approach
was initially developed (>8–10% for the considered bundle aspect
*ratio), i.e., when the number of bundle–bundle contacts per bundle*
is greater or equal to 2 (largely above the percolation
thresh-old), a preliminary study has proved that numerical results were
*not affected by this choice of d. At lower ﬁbre-bundle content,*
both the physics at the bundle scale and the adopted generation
procedure may become questionable so that the size of the REV
should be reconsidered and increased (see for instance Section
4.1).

The generation process permits to obtain three different shapes
for the ﬁbre orientation distribution of bundle angles b of the
*studied planar networks, i.e., uniform, Gaussian-based and *
crenel-lated, the two latter ones being centred on = 0. They are shown in
Fig. 2(a–c). The characteristics of the uniform distribution are that
its amplitude is chosen and that there are no privileged classes of
ﬁbre angles b*(cf.*Fig. 2(a)). The Gaussian-based distribution
con-sists ﬁrst in starting from a Gaussian distribution of orientation
angles bfor ﬁbres, and then in using the -periodicity of with
respect to b*to normalize the resulting histograms (cf.*Fig. 2(b)).
The crenellated distribution is detailed hereafter. It exhibits a peak,
which intensity and amplitude can be varied. More precisely, given
the number N of ﬁbres in the REV, two orientation amplitudes
˛1and ˛2are imposed to two populations of N1and N2= N − N1
ﬁbres, respectively. A random distribution is set for both

popula-tions of ﬁbres, leading to superimpose two random distribupopula-tions
between−˛1/2 and +˛1/2 and between −˛2/2 and +˛2/2,
**respec-tively (ﬁbrous microstructures are oriented in the e1-direction).**
As depicted in the simpliﬁed graph ofFig. 2(c), ﬁbre orientation
in generated REV’s can be characterized by ˛1, the base
orienta-tion amplitude, r˛= ˛2/˛1, the amplitude ratio and rN= N2/N, the
fraction of ﬁbres in the peak exhibited by this type of orientation
*distribution. Notice that at ﬁxed values of N and ˛1*, the increase of
rNis accompanied with an increase of r˛.

In order to detect bundle–bundle contacts, a control volume
Vb *is assigned to each bundle b: every bundle c which *
centre-line intersects Vb *is added to the connectivity set of bundle b.*
The control volume Vbis chosen as a rectangular box with
dimen-sions l × dmax× ı∗_{dmin, where ı}∗_{is a dimensionless parameter}_{[7]}_{.}
In the following, the generated bundle networks will be
*charac-terized by their bundle volume fraction f, and by the second ˜***A**(2)

and fourth ˜**A**(4)2D-orientation tensors. These macroscopic
descrip-tors of the microstructure are respectively deﬁned in a discrete
way by:
f = Ndmaxdminl
4Vre*v* ,
˜
**A**(2)= 1
N
N

### b=1 ˜

**p**

_{b}

**⊗ ˜pb, ˜A**(4)= 1 N N

### b=1 ˜

**p**

_{b}

**⊗ ˜pb⊗ ˜pb⊗ ˜pb.**(30)

*3.3. Computational rheometry*

Two types of calculations will be presented in the following:
*(1) Instantaneous mechanical responses of the generated REV’s*

—Thanks to the linearity property(29), the mechanical response
of a microstructure at a given time can be entirely determined
imposing on the studied REV’s four independent macroscopic
**velocity gradients, i.e., e**_{i}**⊗ ej(i, j ∈ {1, 2}). In practice, given one**
of these four macroscopic velocity gradients, this consists in
inverting the linear system(22)in order to compute (i) the
unknown kinematical ﬁelds

**v**

˜[1]**v**

_{b}and ˙[0]

_{b}, (ii) the overall stress

**tensor of the suspension (according to (26)) and (iii) the rate**

**˙˜A**(2)of the orientation tensor ˜

**A**(2)deﬁned as (according to(28) and (30)):

**˙˜A**(2)= 1 N N

### b=1 ( ˙˜

**p**

_{b}

**⊗ ˜pb+ ˜pb⊗ ˙˜pb).**(31)

*(2) Time-evolution of microstructures —In order to determine the*
time-evolution of a REV during a given mechanical loading,
both a Lagrangian point of view and an explicit time-integration
scheme have been adopted. More precisely, after each “snapshot
* calculation” performed at a given time t, the position x*t+ıt

_{b}of the centre of mass Gb

**as well as the orientation p**t+ıt

_{b}

*of a bundle b*at time t + ıt are updated from the knowledge of the position

**x**t

b**, the orientation p**tband the computed velocity ﬁelds

** v**

[1]
b and
˙[0]
b **v**

**e**3

*at t:*

**x**t+ıt

_{b}

**= x**t b

**+ (L · x**tb+

** v**

[1]
b )ıt
**v**

**p**t+ıt

_{b}

**= p**t b+ ( ˙ [0] b

**e**3

**× p**t

_{b})ıt. (32)

Therewith, the connectivity of the updated REV is achieved following the method given in Section 3.2, and a new time iteration can be achieved. A preliminary study has been per-formed in order to determine the time-step values ıt that give reproducible and time-step insensitive simulations.

**Fig. 2. (a) Uniform ﬁbre orientation distribution ranging between**−60◦_{and 60}◦_{, (b) Gaussian-based ﬁbre orientation distribution, (c) crenellated ﬁbre orientation distribution,}

with their corresponding second-order orientation tensors ˜**A**(2), (d) example of a generated REV (V(s)_{= 25 mm × 25 mm × 2.5 mm) containing 437 bundles of length 25 mm}

(f = 0.188) (symbols represent the connections location, lines represent the mean center-line of the bundles). (e) Same REV after ﬂowing under a unit plane strain deformation until an axial Hencky strain ε33= ln(h/h0)= −1.

In order (i) to underline the role of both the ﬁbrous microstruc-ture (bundle content and orientation) and the loading path on the macroscopic response of the suspension, and (ii) to test the capability of usual ﬁbre orientation models in the concentrated regime, numerical simulations presented below were performed with the following microstructural parameters which values are typical of those encountered in polymer composites (SMC or GMT):

• the dimensions of the bundles were l = 25 mm, dmax= 0.6 mm, dmin= 0.06 mm, and the REV’s are 25 mm × 25 mm × 2.5 mm rectangular boxes[7],

• bundle networks were generated with the procedure described
in Section3.2(Ã_{12}(2)≈ 0). The principal orientation of the networks
Ã_{11}(2)ranged between 0 and 1, the volume fraction of bundles f
between 0.05 and 0.3,

• the thickness ˛ of the equivalent sheared contact prisms was ﬁxed
to 2m, the dimensionless parameter ı∗_{to 3}_{[7]}_{.}

The generated REV’s were subjected to two mechanical loading conditions:

* • a unit plane strain compression (I) in (e1, e3), i.e., a 1D *
elonga-tional ﬂow in

*P:*

**L**_{I}**= e1⊗ e1− e3⊗ e3,** (33)
**• a unit pure shear (II) in (e1, e2***), i.e., an irrotational shear ﬂow in*

*P:*
**L**_{II}=1

2**(e**1**⊗ e2+ e2⊗ e1).** (34)

As an example,Fig. 2(b) gives the deformed shape of the REV plotted inFig. 2(a) after a unit plane strain compression up to an axial Hencky strain ε33= ln(h/h0)= −1.

**4. Instantaneous responses**

The ﬁrst presented simulation results are snapshots in time of
the instantaneous evolution of ﬁbre-bundle networks. The
follow-ing sections aim at describfollow-ing the inﬂuence of the ﬁbre volume
fraction or the inﬂuence of current ﬁbre orientation on the rate of
orientation ˙˜**p**_{b}and on the orientation rate tensor ˙˜**A**(2). This is ﬁrst
*performed using micro–macro modelling predictions (cf. Sections*
4.1 and 4.2*). Then a comparison with usual approaches (cf. Section*
2) is achieved in Sections4.3–4.5.

*4.1. Inﬂuence of the ﬁbre volume fraction on the orientation rate*

Fig. 3(a) gives the evolution of the components ˙Ã(2)_{11} and ˙Ã(2)_{12}
of the tensor ˙˜**A**(2) calculated for nearly isotropic Gaussian-based

microstructures (Ã(2)_{11} ≈ 0.5) and subjected to a 1D elongational
ﬂow.Fig. 3(b) gives the evolutions of the same components for
highly oriented microstructures (Ã(2)_{11} ≈ 0.8) tested for the same
ﬂow kinematics. Whatever the studied microstructure (isotropic
or oriented), we can notice that the ˙Ã(2)_{12} components are very low
compared to the ˙Ã_{11}(2)components.

• For f > 0.05, it appears that the ﬁbre volume fraction has not an important inﬂuence on the results.

• For f ≤ 0.05, the same observation can be made despite a larger scattering of the results. The origin of this scattering is mainly due to the low number of bundles that are present in REV’s, moreover some remote bundles or remote clusters of bundles can be found in the generated REV’s. These elements are not accounted for the calculations of the macroscopic properties of the generated REV’s [7]. Typical sizes of these clusters can be of the same order as the sizes of the REV’s so that the size of the REV’s may be inappropri-ate for such situations. To obtain reliable results two alternatives can be followed: the ﬁrst one consists in increasing the size of the generated REV’s, the second one consists in performing a large number of calculations on REV’s of limited sizes in order to get representative average values of the studied properties[37,38]. Here, this last option was chosen. It has also to be pointed out that remote bundles or clusters could have an impact on the rate of the orientation tensor in this range of rather low ﬁbre vol-ume fractions. In this particular case, the micro–macro approach

**Fig. 3. Inﬂuence of the ﬁbre volume fraction f on the rate of the components of the orientation tensor ˜A**(2)for 1D elongational ﬂows (a and b) and for pure shear ﬂows (c
and d) in*P- (a) and (c): nearly isotropic REV’s (Ã*(2)

11 **≈ 0.5) - (b) and (d): highly oriented REV’s along e**1(Ã(2)11≈0.8). Calculations are performed using Gaussian-based ﬁbre

**Fig. 4. Components ˙p**i**of the orientation evolution vector ˙p**bfor each ﬁbre-bundle of REV’s having a number of ﬁbre-bundles N = 600. Comparison between micro–macro

(symbols) and “Jeffery”(lines) predictions for 1D elongational ﬂows in* P along e*1. Calculations are performed using uniform ﬁbre orientation distributions. (a) Nearly isotropic

- f = 10%, (b) highly oriented - f = 10%, (c) nearly isotropic - f = 25%, (d) highly oriented - f = 25%.

should be improved by accounting for bundle–ﬂuid interactions in order to incorporate the inﬂuence of these remote elements or domains in the description of the rheological behaviour of the suspension.

• When these microstructures are subjected to a pure shear
kine-matics (Fig. 3(c) and (d)), the same trends are observed.
•Fig. 4 (a–d) shows the components of ˙˜**p**_{b} obtained by the

micro–macro approach for each bundle of nearly isotropic and
very oriented cells subjected to 1D elongational ﬂows. Two
ﬁbre-bundle fractions (f = 10% and 25%) are considered. These ﬁgures
also underline the strong inﬂuence of the global orientation
*what-ever the ﬁbre fraction f. For a given orientation, clouds of points*
represented in these ﬁgures are close when comparing the two
tested ﬁbre-bundle fractions. Nonetheless, it has to be noticed
*that the dispersion of results decreases when increasing f: i.e., the*
clouds of points is more compact for high bundle fractions. These
observations have to be related to the decrease of the dispersion
of the components of ˙˜**A**(2)ofFig. 3(a–d).

• Thus, given the very weak inﬂuence of the ﬁbre volume fraction
f on the components of **˙˜A**(2)for elongational and shear ﬂows for

f > 0.05, we will focus the rest of our study on differently oriented microstructures with an identical ﬁbre content of 0.2.

*4.2. Inﬂuence of the current orientation of ﬁbres on the*
*orientation rate*

First results of Fig. 5 (a) and (b) are obtained from
calcula-tions performed using cells where the ﬁbre orientation distribution
is Gaussian-based. InFig. 5(a), the components of ˙˜**A**(2) are given
as a function of the current orientation Ã(2)_{11} for cells having
dif-ferent ﬁbre orientations subjected to an elongational kinematics
(f = 0.2). Micro–macro predictions show that the orientation rate
in the ﬂow direction (given by ˙Ã_{11}(2)) strongly depends on the
cur-rent ﬁbre orientation, which is given here by Ã(2)_{11}. The maximum of
ﬁbre orientation evolution in the direction of the ﬂow is obtained
for nearly isotropic structures (Ã(2)_{11} ≈ 0.5) and this decreases with
**the ﬁbre orientation intensity, either in the e1-direction or in the**

**e**2-direction. It is interesting to notice that the evolution of ˙Ã_{11}(2)is
not exactly symmetrical with respect to Ã(2)_{11} = 0.5: the decrease of

**Fig. 5. Inﬂuence of the orientation intensity Ã**(2)_{11} on the components of the orientation tensor rate ˙˜**A**(2): (a) for 1D elongational ﬂows in* P along e*1, (b) for pure shear in the

case of Gaussian-based ﬁbre orientation distributions, (c) and (d) are respectively the same as (a) and (b) in the case of uniform ﬁbre orientation distributions. Comparison between micro–macro and “Jeffery” predictions.

˙Ã(2)
11 is higher when Ã
(2)
11 < 0.5 than when Ã
(2)
11 ≥ 0.5. Notice that
Ã(2)_{11} has nearly no inﬂuence on ˙Ã(2)_{12}. Even if it is never exactly zero,
it remains small compared to ˙Ã(2)_{11}. This can simply be attributed
to the random generation process where the average alignment of
**ﬁbres along e**1is never perfect.

Fig. 5(b) represents the same kind of results for oriented REV’s
subjected to pure shear kinematics. In this case, the ﬁrst principal
value ˙Ã_{I}(2)and the value of the angle between the major principal
**vector e**I**and the direction e1**of ˙˜**A**

(2)

are represented with respect
to Ã(2)_{11}. The micro–macro predictions show that this angle is close
to /4 whatever the current ﬁbre orientation given by Ã(2)11. Hence,
even if the subjected kinematical loading is irrotational, the ﬁbrous
microstructure rotates. The maximum of ˙Ã(2)_{I} is obtained for cells
**highly oriented either in the e1-direction or in the e2-direction.**
Moreover, this evolution appears to be symmetrical with respect
to Ã(2)_{11} = 0.5 in this case.

Fig. 5(c) and (d) give respectively the same type of results as
Fig. 5(a) and (b) for calculations performed using uniform ﬁbre
orientation distributions. General trends are quite close to the
pre-vious ﬁgures. Nevertheless, the evolution of ˙Ã(2)_{11} (respectively ˙Ã_{I}(2))
exhibits a more complex “wavy” shape with two local maxima

(respectively minima) for the elongational kinematics (respectively
the pure shear) than in the case of the Gaussian-based
*calcula-tions. Moreover, the obtained rates can differ quite largely too, e.g.,*

˙Ã(2)

11 ≈ 0.3s−1at Ã (2)

11 = 0.35 for the uniform distributions whereas ˙Ã(2)

11 ≈ 0.24 s−1 for the Gaussian-based case and 1D elongational ﬂows. Thus, it appears that the shape of the ﬁbre orientation distribution is preponderant on the rate of the evolution of the orientation of ﬁbres whatever the tested kinematics.

This important observation is conﬁrmed when using
crenel-lated ﬁbre orientation distributions as depicted in Fig. 6(a) for
elongational kinematics. This ﬁgure indicates that the rate of the
components of the second-order orientation tensor will “slow
down” as the fraction ﬁbres rN *of ﬁbres will decrease, i.e., when*
the orientation distributions exhibit sharp orientation peaks. As
evident from the graph ofFig. 6(c), for cells having a similar
aver-age valueÃ(2)

11 of the orientation tensor (Ã (2)

11 ∈ [0.64, 0.68]), a very
large scattering of the orientation rates can be induced by changing
the orientation parameters rNand r˛: 0.17 s−1< ˙Ã_{11}(2)<0.33 s−1. This
ﬁgure shows that the lower the number fraction rN*, i.e., the sharper*
the peak shape, then the lower the orientation rate ˙Ã_{11}(2). This trend
is systematically observed for other orientation statesÃ(2)

11 > 0.5. It can also be noticed that calculations carried out with

**crenel-Fig. 6. Inﬂuence of the orientation intensity Ã**_{11}(2)on ˙Ã(2)_{11}, for 1D elongational ﬂows in* P along e*1. (a) Comparison of the micro–macro predictions in the cases of uniform,

Gaussian-based or crenellated ﬁbre orientation distributions with the predictions of the hybrid and natural closure approximations, (b) same type of comparison when using
this time the Jeffery predictions instead of the micro–macro ones. Remark: only polynomial best ﬁts of the simulation results are given to make the ﬁgures readable. (c)
Evolution of ˙Ã_{11}(2)for the micro–macro approach with respect to rN(˛1= , 0 < r˛< 1, REV’s with a similar average orientation such that Ã(2)11∈ [0.64, 0.68]).

lated ﬁbre orientation distributions with rN> 0.8 are naturally
close to the results obtained for uniform orientation distributions.
A simple rule therefore can be established: ﬁbre orientation
*distri-butions which exhibit some peaks, i.e., like the Gaussian-based or*
crenellated orientation distributions, will give slower rates for the
orientation evolution than the uniform distribution. The relevance
of a particular type of ﬁbre orientation distributions is investigated
in Section5.

*4.3. Inﬂuence of the current orientation of ﬁbres on the*
*orientation rate tensor using “Jeffery” predictions*

Results given inFig. 5were also obtained for simulations called
“Jeffery” simulations. The “Jeffery” simulations consisted in
calcu-lating the rate of orientation change of each generated single ﬁbre
of the tested cells adopting Jeffery’s Eq.(1)and then using these
data to calculate the components of the orientation rate tensor
**˙˜A**(2)according to Eq.(31). Notice that another equivalent approach
would have consisted in performing a calculation of Eq.(10), which
is only the rewritten Jeffery equation for the rate of the
second-order orientation tensor, using a discrete evaluation of ˜**A**(2)and ˜**A**(4).
It was checked that both ways of calculation gave similar results.

In a sense, our approach could be seen as using an exact closure
approximation for ˜**A**(4)in the expression for ˙˜**A**(2)given by Eq.(10).

When comparing this approach to the micro–macro
computa-tions one can check that the predicted trends are, at a ﬁrst sight,
very similar, which might seem surprising. This observation holds
whatever the tested orientation Gaussian-based and uniform
distri-butions. For the pure shear case, the shape of the both predictions
are very close all over the orientation range. For the elongational
ﬂow, it is interesting to notice that both approaches do not match
exactly. If the Jeffery prediction gives a symmetrical evolution with
respect to Ã_{11}(2)= 0.5, this is no more the case of results predicted
by the micro–macro approach. This is particularly evident for rather
oriented networks (Ã(2)_{11} > 0.7) along the ﬂow direction. This
differ-ence should be further studied, but could possibly be attributed to
the pronounced anisotropy of the ﬁbrous medium in these
*situa-tions: e.g., the Jeffery equation considers the case of the orientation*
evolution of a remote ﬁbre immersed in a isotropic viscous medium,
but here the situation is largely different and one would rather have
to consider the case of a ﬁbre immersed in an anisotropic medium
[22]. It should be also pointed out that the inﬂuence of local
inter-action moments might increase, as shown in Le Corre et al.[7]for
these particularly oriented microstructures. They might possibly

become no more negligible at the macroscopic level. Accounting for their effects in the micro–macro approach could be possible: this would lead to an equivalent description of the rheological behaviour of the suspension, which would be a general Cosserat medium, as shown theoretically in[6].

Fig. 4(a–d) allows comparing the components of ˙˜**p**_{b}given for
individual cells by the micro–macro and the Jeffery approaches.
Predicted shapes of the clouds of points given by the micro–macro
approach are quite close to the Jeffery prediction, whatever the
ﬁbre-bundle fractions and orientations, but the micro–macro one
depicts a more complex situation than the Jeffery one. Indeed, all
results of the micro–macro approach appear to be dispersed around
the lines given by using the Jeffery theory. This is especially the
case of nearly isotropic microstructures, but it seems that bigger
differences can be observed when the microstructures are highly
oriented. This latter result has to be linked with the previous
obser-vation on the evolution of the components of ˙˜**A**(2).

Jeffery predictions are also close to the micro–macro ones for crenellated orientation distributions as it appears when comparing Fig. 6(a) and (b). Thus, the relative accuracy of the Jeffery prediction with respect to the micro–macro one (except for highly oriented microstructures) seems to be a general rule.

*4.4. Inﬂuence of the current orientation of ﬁbres on the*
*orientation rate tensor using closure approximations*

Results ofFig. 7are obtained for Gaussian-based ﬁbre
orien-tation distributions. They enable to compare the predictions for
the evolutions of the components of the orientation rate tensor
**˙˜A**(2) given by the micro–macro approach with the predictions of
usual modelling approaches using closure approximations in Eq.
(10)for 1D elongational and pure shear kinematics. As in Section
4.3, the Jeffery approach is also placed in those ﬁgures for
com-parison. Whatever the tested kinematics, the following points are
worth being noted:

• For isotropic states of ﬁbre orientation (Ã(2)

11close to 0.5), the linear closure approximation gives quite good predictions when com-pared to the micro–macro ones. This result was expected as the linear closure approximation is exact for isotropic orientation states if every ﬁbre rotates according to Jeffery’s equation (see

*e.g.*[9]). Nonetheless, the predicted orientation rate appears to
be insensitive to current orientation intensity, which is a serious
drawback. For instance, this approximation does not predict that
the orientation decreases for very oriented states and therefore
seems to seriously fails.

• At the opposite, the quadratic closure approximation largely
overestimates the ˙Ã(2)_{12} and ˙Ã_{11}(2)for both tested kinematics and
isotropic orientation and is therefore adapted to very oriented
states only. As previously, this latter result was also expected as
the quadratic closure is exact for any aligned orientation states if
*every ﬁbre rotates according to Jeffery’s equation (see e.g.*[9]).
• The hybrid and natural closure approximations follow correctly

the trends given by the micro–macro approach and by Jeffery’s
type calculations. Their predictions are good for isotropic and
very oriented states and a certain discrepancy is observed for
intermediate regimes, depending on the mechanical loading path.
• Whatever the tested kinematics, usual modelling approaches
pre-dict that the evolution of the components of ˙˜**A**(2)is symmetrical
with respect to the isotropic ﬁbre orientation state. If this
symme-try is observed for the micro–macro approach in the case of the
pure shear kinematics, this is not the case, as we have previously
noticed it, for the 1D elongational kinematics.

Likewise, predictions for the components of **˙˜A**(2) of the
hybrid and natural closure approximations are compared to the
micro–macro and Jeffery results for crenellated and uniform ﬁbre
orientation distributions inFig. 6 for the 1D elongational
kine-matics. Whatever the tested orientation distributions, none of
those closure approximation gives results corresponding to the
micro–macro or Jeffery results over the whole range investigated for

˜

**A**(2). Nevertheless, it can be observed that these two closure
approx-imations give trends that belong to the large spectrum of possible
evolution rates that can be reached for all the possible orientation
distributions and orientation intensities.

To summarize, no closure approximation compares with the micro–macro approach like the Jeffery-type approach, whatever the tested orientation distributions and the kinematics, which are not exhaustively presented here. It should be noticed that the com-putation of the Jeffery approach induces an exact calculation of

˜

**A**(4) in a discrete way (see also the remark given at the
begin-ning of the previous section). Thus, the Jeffery approach, which

**Fig. 7. Inﬂuence of the orientation intensity Ã**(2)

11on the components of the orientation tensor rate ˙˜**A**
(2)

: (a) for 1D elongational ﬂows in* P along e*1, (b) for pure shear. Calculations

adopts a mean ﬁeld assumption for the macroscopic velocity ﬁeld,
seems to be the most relevant when compared to the micro–macro
one. Nevertheless, none of those approaches explains the observed
discrepancy for elongational ﬂows of oriented ﬁbre networks
(Ã(2)_{11} > 0.7).

*4.5. Hydrodynamic diffusion terms*

As mentioned in Section2.4, corrective terms, known as
hydro-dynamic diffusion terms, have been added by several authors in
order to account for the ﬁbre–ﬁbre interactions, in the case
semi-dilute of suspensions [25,27]. In this section, we compare the
predictions of the micro–macro approach with those of the Jeffery
approach using a similar technique to compute ˙˜**A**(2)as in Sections
4.3 and 4.4, but adding one term, which accounts for the
hydro-dynamic diffusion. All tested microstructures of this section have
Gaussian-based orientation distributions. One of the simplest
dif-fusion model proposed in the literature by Phan-Thien et al.’s (PT)
is chosen here. This diffusion term implies to use an interaction
coefﬁcient, which is written as[27]:

CI= 0.03(1 − exp(−0.224fr)). (35)

Here, this coefﬁcient is equal to CI= 0.0251 for f = 0.2. It is impor-tant to make the following remarks concerning this model. • On the contrary to this model, it has to be noticed that no

inﬂu-ence of the ﬁbre volume fraction f (f ≥ 0.05) is revealed by the micro–macro approach.

**• Adding this term to the equation for the evolution of ˙˜A**(2)leads to
break its linearity (as previously mentioned in Section2) on the
contrary to the simplest Jeffery or micro–macro predictions.

As clear fromFig. 8, the interaction coefﬁcient inﬂuence is not
consistent with the trends obtained by the micro–macro approach
for the studied concentrated suspensions. InFig. 8(a), the
orienta-tion rate for ˙Ã(2)_{11} is overestimated for low orientation whereas it is
underestimated for high orientation for 1D elongational ﬂow cases.
Thus, it seems that the increase of the orientation rate observed for
highly oriented microstructures in the direction of the 1D
elon-gation cannot be described by this type of interaction coefﬁcient.
*For pure shear loading (cf.*Fig. 8(b)) the evolution of ˙Ã_{12}(2)is well

predicted, but the evolutions of ˙Ã(2)_{11}, which are obtained by the
micro–macro or PT approaches are drastically different. In the case
of the PT model, ˙Ã(2)_{11}decreases as Ã(2)_{11}increases, whereas it remains
close to zero in the case of the micro–macro approach. This
obser-vation means that both predictions will give completely different
principal orientation axes for the 2D second-order orientation
ten-sor ˜**A**(2).

**5. Time-evolution of ﬁbre orientation**

The evolution of ﬁbrous microstructures subjected for 1 s to a 1D elongational ﬂow (constant plane strain compression at 1 s−1, see (33)) is now analyzed. Notice that simulations were performed with a reliable time-step of 10−2s. Also notice that such ﬂow conditions correspond to a REV height reduction of about 65 %, which is close to typical processing conditions. Two different methods were used to compute the evolution of ﬁbre orientations and spatial positions within the tested REV’s:

• The ﬁrst method consisted in performing “direct” calculations, by integrating step by step with Eq.(32)the ﬁbre orientation and spatial position of each ﬁbre contained in REV’s. This was done by using the micro–macro and the Jeffery-type approaches. For the ﬁrst approach, the translation ε

**v**

[1]**v**

_{b}and rotation ˙[0]

_{b}veloc-ity ﬁelds were obtained by solving the localization problem(22). For the second approach, the rotation velocities ˙[0]

_{b}were com-puted with Jeffery’s Eq.(1), and the ε

**v**

[1]**v**

_{b}’s were set to 0 (afﬁne motion of ﬁbres). The initial ﬁbrous microstructures displayed random ﬁbre positions and three Gaussian-based distributions

**of ﬁbre orientation, aligned in the e**1-direction and which ini-tial orientation tensors were such that Ã

_{11}(2)

_{= 0.25, 0.5 and 0.75,}respectively. All results, that were averaged over 20 REV’s with the same microstructural parameters, are presented inFig. 9, which gives the evolutions of Ã

_{11}(2), ˙Ã

_{11}(2), Ã(2)

_{12}and ˙Ã(2)

_{12}with respect to time (a) and Ã(2)

_{11}(b), respectively.

• The second method, also carried out with the same initial
microstructures, assumed that the positions of ﬁbres always
remained randomly spatially distributed in the REV’s, and that
the orientations of ﬁbres always exhibited Gaussian-based
distri-butions. In order to compute the evolution of ﬁbre orientation,
the values of ˙Ã(2)_{11} were obtained from polynomial ﬁts of the data

**Fig. 8. Inﬂuence of the orientation intensity Ã**(2)

11 on the components of the orientation tensor rate ˙˜**A**
(2)

**: (a) for 1D elongational ﬂows along e**1, (b) for pure shear. Calculations

**Fig. 9. Average orientation evolution in time for 20 different cells with initially Gaussian-based distributions: planar compression test along e**1with D11= −D33= 1 s−1,

N = 500 ﬁbres: (ai) ˜**A**
(2)

components versus time, (bi) ˙˜**A**
(2)

components versus Ã(2)

11- initial value of Ã (2)

plotted inFigs. 7(a) and8(a). Results deduced from this method have also been reported inFig. 9(the so-called “ﬁt” results). • Likewise,Fig. 11displays results obtained by the ﬁrst method for

the micro–macro and Jeffery calculations. Results called “hybrid”
and “natural” are given by adopting the second method described
in the previous point. The values of ˙Ã(2)_{11} are ﬁtted from the data of
Fig. 7for the natural and hybrid closure approximations. Here, an
average initial orientation of the tested microstructures is taken
*into account, i.e., Ã*_{11}(2)= 0.5.

• At last,Fig. 12shows similar results for initially crenellated
ori-entation distributions with approximately the same value of
Ã_{11}(2)≈ 0.65, but various orientation parameters rN and r˛. The
time-evolution is computed following the two approaches of the
previous “ﬁrst” method (lines with points for the micro–macro
approach, and continuous lines for Jeffery’s approach). A third
approach of the time-evolution of the tested microstructures is
also used (continuous lines with triangles): it consists in
adopt-ing the Jeffery’s approach to compute the orientation rate ˙_{b}[0]
of each ﬁbre and incorporating the translation ﬁeld ε

**v**

[1]**v**

_{b}of each ﬁbre in Eq.(32): this third approach therefore adopts a non-afﬁne velocity ﬁeld.

The graphs plotted in these ﬁgures conjure up the following comments:

• Whatever the initial ﬁbrous microstructures and the method
adopted to compute the evolution of ﬁbre orientation, ﬁbrous
**net-works align in the e**1-direction during the ﬂow: Ã11(2)increases and
Ã_{12}(2)remains very close to 0.

• As already pointed out in the previous section, when
assum-ing randomly distributed ﬁbres with Gaussian-based orientations
(“ﬁt” results), predictions given by Jeffery’s equation or by the
micro–macro approach are very close, except for ﬁbrous networks
**that are highly oriented in the e**1-direction (Fig. 9(a3) and (b3)).
On the contrary, predictions given with the diffusion coefﬁcient
(PT “ﬁt” results) systematically deviate from the two previous
types of simulation: the ﬁbre orientation is slowed down for
ini-tially random or aligned microstructures (Fig. 9(a2,b2,a3,b3)), but
**it is enhanced when ﬁbres are initially aligned in the e2-direction**
(Fig. 9(a1,b1)).

• Whatever the initial ﬁbre orientation, predictions given by
the ﬁrst calculation method (micro–macro or Jeffery) always
differ from those given by the second method (“ﬁt” results,
micro–macro or Jeffery). In order to analyze more closely such
a discrepancy, we plotted inFig. 10the average orientation
distri-bution functions that were obtained at the end of the simulations
with the ﬁrst method (micro–macro or Jeffery). We also
plot-ted in the same ﬁgure the orientation distribution functions of
REV’s having the same second-order orientation tensors but with
*Gaussian-based orientation distributions, i.e., similar to those that*
were used with the second method. As evident from this
ﬁg-ure, the ﬁbre orientation within ﬂow-induced microstructures
(method 1) severely differs from the Gaussian type orientation
distribution: they may exhibit more than one preferential
ori-entation peak (seeFig. 10(a)), and the corresponding peaks are
sharper. It has to be noticed that this type of ﬁbre orientation
distributions have a shape quite close to the crenellated
orien-tation distributions tested in the previous section. It has been
observed that developing sharp orientation peaks in the ﬁbre
ori-entation distribution has for effect to decrease the oriori-entation
rate ˙Ã_{11}(2). This observation may explain the strong decrease of the
orientation rate ˙Ã(2)_{11} observed inFig. 9(b1–b3).

• For the investigated ﬂow conditions,Fig. 9also shows that the Jeffery’s equation and the micro–macro approaches for

**ﬂow-Fig. 10. Average orientation distributions for 20 different cells. Comparison of**

time-evolution calculations and initial Gaussian-based distributions with the same
average orientation: (a) initial Ã(2)_{11} ∼= 0.25, (b) initial Ã(2)

11 ∼= 0.50, (c) initial Ã (2) 11 ∼=

**Fig. 11. Comparison of time-evolution calculations using the micro–macro and the Jeffery approaches, as well as the hybrid and natural closure approximations for 1D**

elongational ﬂows in* P along e*1: (a) Ã(2)

_{11}with respect to time, (b) ˙Ã

_{11}(2)with respect to Ã(2)

_{11}, for initial random orientation (Ã(2)

_{11}(t = 0) ∼= 0.50). induced microstructures give, at ﬁrst approximation, nearly the

same results concerning the second-order orientation tensor during the simulations. This remark is strengthened by the graphs ofFig. 10: the corresponding orientation distribution func-tions are rather close. The observed differences, which are very weak, are much pronounced for initially oriented microstructures (Figs. 9(b1) and 10(a)). They may be ascribed to a loss of the initial random positions of ﬁbres when using the micro–macro approach, since in this case ε

**v**

[1]**v**

_{b}

**/= 0.**•Fig. 11shows that the natural closure approximation gives results very close to the Jeffery predictions. This was expected as this closure approximation was particularly developed to be exact when starting with an isotropic orientation, and if every ﬁbre rotated according to Jeffery’s equation. It must be pointed out that this result holds only for this particular case of ﬁbre ori-entation and is not a general rule. On the contrary, the hybrid closure results are not in accordance with the evolution predicted

**Fig. 12. Evolution of ˙Ã**_{11}(2)with Ã_{11}(2)for initially crenellated ﬁbre distributions (1D
elongational ﬂows in* P along e*1).

by the micro–macro or Jeffery-type approaches, the orientation state and the evolution rates are overestimated.

• Lastly, the continuous lines plotted in the graph ofFig. 12prove
that Jeffery’s approach proposes reasonable predictions, at ﬁrst
approximation, of ﬁbre orientation within the considered
con-centrated bundle suspensions even for initially crenellated ﬁbre
orientation distributions. By looking at the continuous line with
the triangles, also notice that the prediction can be improved if
*the third approach (cf. above) of time-evolution simulations is*
*used, i.e., when adopting a non-afﬁne velocity ﬁeld.*

**6. Conclusion**

*A micro–macro approach, i.e., a discrete homogenization*
technique, is used to study the rheological behaviour of very
concentrated suspensions seen as connected planar networks of
ﬁbre-bundles with Newtonian viscous interactions. The numerical
tool, which was developed on the basis of this theoretical approach,
enables to generate ﬁbre-bundle networks having various
*orien-tation distributions: i.e., Gaussian-based, uniform and crenellated*
orientation distribution functions. These networks can be subjected
to any kind of mechanical loadings. In this work, 1D elongational
and pure shear ﬂows were used. It is thus possible to analyze the
inﬂuence of microstructural parameters such as the ﬁbre-bundle
content or the ﬁbre-bundle orientation on the evolution of the
ori-entation state.

*Results obtained from instantaneous tests ﬁrst show that there is*
no inﬂuence of the ﬁbre-bundle volume fraction on the orientation
evolution in the concentrated regime, which is studied here. On the
contrary, for a given type of orientation distribution, the mean
aver-age orientation given by the second-order orientation tensor, has
a strong impact on the orientation rate. Changing the type of
ori-entation distributions has also a drastic effect. For 1D elongational
ﬂows, a rule seems to emerge from the set of results: the sharper the
peak exhibited by the orientation distribution, the lower the rate of
orientation evolution. In spite of the completely different physics of
both approaches, it is also shown that Jeffery’s predictions can be
well compared to the micro–macro results even if some
discrepan-cies are found for microstructures aligned along the ﬂow direction.
Closure approximations are rather deﬁcient. They are only relevant
for some particular cases of orientation states. In the same way, the
approach using a hydrodynamic diffusion term is deﬁcient as well,
and has also the disadvantage of losing the linearity of the rate of